Mode I Critical Stress Intensity Factor of Medium Density Fiberboard Obtained by SingleEdge Notched Bending Test


 Lynne McKenzie
 2 years ago
 Views:
Transcription
1 ... Yoshihara, Mizuno: Mode I Critical Stress Intensity Factor of MediumDensity... Hiroshi Yoshihara, Hikaru Mizuno 1 Mode I Critical Stress Intensity Factor of Medium Density Fiberboard Obtained by SingleEdge Notched Bending Test Faktor kritičnog intenziteta naprezanja (I. mod) MDF ploča dobiven testom savijanja Original scientific paper Izvorni znanstveni rad Received prispjelo: Accepted prihvaćeno: UDK: 630* ; 630*812.71; doi: /drind ABSTRACT The Mode I critical stress intensity factor (K Ic ) obtained by singleedgenotched bending (SENB) tests of mediumdensity fi berboard (MDF) was experimentally analyzed. In the SENB test, the critical load for crack propagation (P c ) was determined from the relationship between load/loadingline displacement and load/crack opening displacement (COD). A double cantilever beam (DCB) test was also conducted and the results were compared with those of SENB tests. The value of Mode I critical stress intensity factor was obtained by introducing an additional crack length, when the crack length ranged from 0.5 to 0.7 times the depth of the specimen. This range coincided well with that used to derive the appropriate K Ic value in the singleedgenotched tension (SENT) test, which was conducted using the specimens with a similar configuration cut from the MDF panel used in this study. Key words: additional crack length, Mode I critical stress intensity factor, mediumdensity fiberboard (MDF), western hemlock, singleedgenotched bending (SENB) test SAŽETAK U radu se eksperimentalno analizira faktor kritičnog intenziteta naprezanja (I. mod) (K Ic ) dobiven testom savijanja s jednim rubnim urezom (SENB) za ploče vlaknatice srednje gustoće (MDF ploče). U SENB testu kritično opterećenje za širenje pukotine (P c ) određeno je iz odnosa opterećenja i linije pomaka te iz odnosa opterećenja i širenja pukotine (COD). Proveden je i dvostruki konzolni test (DCB), a rezultati su uspoređeni s rezultatima SENB testova. Vrijednost faktora kritičnog intenziteta naprezanja (I. mod) dobiven je uvođenjem dodatne duljine pukotine kada je duljina pukotine u rasponu od 0,5 do 0,7 debljine uzorka. Taj se raspon podudario s rasponom koji se koristi za dobivanje odgovarajuće K IC vrijednosti u tenzijskom testu s jednim rubnim urezom (SENT), a proveden je na uzorcima slične konfiguracije izrađenima od MDF ploče koja je upotrijebljena i u ovom istraživanju. Ključne riječi: dodatna duljina pukotine, faktor kritičnog intenziteta naprezanja (I. mod), ploče vlaknatice srednje gustoće (MDF), test savijanja s jednim rubnim urezom (SENB test) 1 Authors are professors at Faculty of Science and Engineering, Shimane University, Matsue, Shimane, Japan. 1 Autori su profesori Fakulteta prirodoslovlja i inženjerstva, Shimane sveučilište, Matsue, Shimane, Japan. DRVNA INDUSTRIJA 65 (2) (2014) 99
2 Yoshihara, Mizuno: Mode I Critical Stress Intensity Factor of MediumDensity INTRODUCTION 1. UVOD In analyzing the fracture behavior of material based on fracture mechanics theory, the value of critical stress intensity factor K c is often measured because it can be regarded as a material constant. Of the three independent fracture modes, the crack opening mode (Mode I) is regarded as more important than the inplane shear mode (Mode II) and outofplane shear mode (Mode III) because the Mode I critical stress intensity factor (K Ic ) is usually smaller than those of Mode II and Mode III, K IIc and K IIIc, respectively. To determine the K Ic value, singleedgenotched bending (SENB), singleedgenotched tension (SENT), compact tension (CT), and double cantilever beam (DCB) tests, the diagrams of which are shown in Figures 1(a) (d), respectively, are most frequently performed because the crack propagation under the opening mode can be easily induced by these tests. In previous works, the K Ic value of mediumdensity fiberboard (MDF) was examined by SENT and CT tests (Yoshihara, 2010b; Yoshihara and Usuki, 2011). In these tests, we found that the K Ic value of MDF can be effectively measured when considering the additional crack length ahead of the crack tip and restricting the range of initial crack length with respect to the specimen geometry. Nevertheless, these tests require attachments to apply the tensile load, so the use of the attachments often restricts the specimen geometry. The SENB test is attractive because it can be conducted using specimens with various geometries more easily than the SENT and CT tests (Yoshihara, 2010a). In this study, we examined the K Ic value of MDF by the SENB test using two types of specimens with different dimensions. The results were compared with those obtained from the DCB tests, which can be determined based on energy consideration and are mathematically well defined (Adams et al., 2003). 2 MATERIALS AND METHODS 2. MATERIJALI I METODE 2.1 Materials 2.1. Materijali An MDF panel, which was used in previous works (Yoshihara, 2010b; Yoshihara and Usuki, 2011), was investigated. The density of the MDF at 12 % moisture content (MC) was 580 ± 10 kg/m 3. The panel was stored in a room at a constant 20 C and 65 % relative humidity (RH) before the test, and the specimens were confirmed to be in an airdried state. These conditions were maintained throughout the tests. Five specimens were tested for each test condition. P a W L = 4W (a) SENB test (b) SENT test (c) CT test (d) DCB test Figure 1 Typical Mode I fracture tests Slika 1. Tipični testovi loma drva I. moda 100 DRVNA INDUSTRIJA 65 (2) (2014)
3 ... Yoshihara, Mizuno: Mode I Critical Stress Intensity Factor of MediumDensity SENB tests 2.2. SENB testovi Figure 1(a) shows the diagram of the SENB test. Two kinds of specimens were tested. Specimen A had dimensions of mm 3, while these dimensions were mm 3 in specimen B. The specimen depth W was 20 and 40 mm in specimens A and B, respectively. The crack was first cut with a band saw (thickness = 1 mm) and then extended 1 mm ahead of the crack tip with a razor blade. The crack length a varied from 1 to 18 mm at intervals of 1 mm in specimen A, and from 2 to 36 mm at intervals of 2 mm in specimen B. Thus, the value of a/w varied from 0.1 to 0.9 at intervals of 0.1. The specimen configurations were similar with those of SENB tests for western hemlock (Yoshihara, 2010a). In the SENB test of western hemlock, the nonlinearity in the relationship between the load (P) and loadingline deflection (δ) was not significant until the init iation of crack propagation, so the critical load for crack propagation was determined as the maximum load (Yoshihara, 2010a). From the results of the SENT and CT tests of MDF in which the crack opening displacement (COD) was measured, the nonlinearity was marked in the PCOD relationship (Yoshihara, 2010b; Yoshihara and Usuki, 2011). Although the loadingline displacement in the SENB test is significantly larger than that in the SENT and CT tests, we thought that the measurement of the COD was effective to detect the nonlinearity and δ. To measure the COD, a clip gauge extensometer (capacity = 5 mm; UB5, Tokyo Sokki, Co., Tokyo, Japan) was used. The specimen was symmetrically supported and loaded at the midspan. The span lengths (L) were 80 and 160 mm in specimens A and B, respectively, giving an L/W value of 4. A steel platen was placed between the specimen and the support to reduce indentation at the supporting point. The load P was applied at a crosshead speed of 0.5 mm/ min 1 until the load markedly decreased. The total testing time was approximately 5 min. Figure 2 shows typical Pδ and PCOD relationships obtained by the SENB tests. In the results for western hemlock, the crack often propagates unstably when the initial crack length is less than 0.3 times the depth of the specimen, whereas it propagates stably when the initial crack is longer than 0.4 times the depth (Yoshihara, 2010a). In the results of MDF, however, the crack always propagates stably all over the range of the initial crack length. In addition, the Pδ and PCOD relationships were significantly nonlinear before the load reached its maximum. Therefore, the critical load for crack propagation P c was provisionally determined to be the load at the onset of nonlinearity. This was determined in the same manner as that used for the SENT and CT tests (Yoshihara, 2010b; Yoshihara and Usuki, 2011) and for the DCB tests described below. Similar to the previous investigation (Yoshihara 2010a), the K Ic value was initially evaluated using the following two equations, which were originally proposed by Gross and Srawley (1965) and Srawley (1976): (1) (2) where B is the beam width Load /, N a/w = 0.1 a/w = 0.3 a/w = 0.5 a/w = 0.7 a/w = 0.9 Load /, N a/w = 0.1 a/w = 0.3 a/w = 0.5 a/w = 0.7 a/w = Loadingline displacement /, mm Crack opening displacement /, mm Figure 2 Typical example of the relationship between load P and loadingline displacement δ and that between P and the crack opening displacement COD for various crack lengths a in SENB test. Depth of the specimen W = 40 mm Slika 2. Tipičan primjer odnosa između opterećenja P i pomaka linije opterećenja δ te između opterećenja P i širenja pukotine COD za različite duljine pukotine a u SENB testu; debljina uzorka W = 40 mm DRVNA INDUSTRIJA 65 (2) (2014) 101
4 Yoshihara, Mizuno: Mode I Critical Stress Intensity Factor of MediumDensity DCB tests 2.3. DCB test The K Ic value was measured by the DCB test using a sidegrooved specimen independent of the SENB test, and it was compared with those obtained from the SENB test. The details of the DCB test were similar to those previously conducted (Yoshihara, 2010a, b). 3 RESULTS AND DISCUSSION 3. REZULTATI I RASPRAVA Figure 3 shows the K Ic a/w relationships obtained from the SENB tests using Eqs. (1) and (2) and a comparison of these relationships with the results obtained by the DCB tests. A convex trend was identified in these relationships. This trend is different from that obtained by the SENB tests of western hemlock. That trend was almost constant in the a/w range of and when using Eqs. (1) and (2), respectively (Yoshihara, 2010a). The K Ic value obtained from specimen A is larger than that from specimen B when comparing the same a/w value, except for a/w = 0.1, so the K Ic values obtained from Eqs. (1) and (2) are regarded to be dependent on the specimen geometry. The point at the onset of nonlinearity, the load at which it was provisionally defined as the critical load for crack propagation P c, could be found earlier in the PCOD relationship than in the Pδ relationship. Therefore, the K Ic value obtained from the PCOD relationship is smaller than that obtained from the Pδ relationship. Figure 3 suggests that the K Ic values obtained using Eq. (1) and (2) are definitively smaller than that obtained by the DCB test because the development of a softened region ahead of the crack tip, such as fracture process zone (FPZ), is not taken into account in these equations. Due to the softened region, the cracked specimen often behaves as if the crack were longer than the actual length. Similar to the approach adopted in previous investigations (Yoshihara, 2010a, b; Yoshihara and Usuki, 2011), the relationship between K Ic and a is modified by introducing an additional crack length into Eqs. (1) and (2) as follows: Figure 3 Comparison of the relationships between K Ic and a/w obtained by SENB test and that obtained by DCB test Slika 3. Usporedba odnosa između K Ic i a/w dobivenoga SENB testom i DCB testom 102 DRVNA INDUSTRIJA 65 (2) (2014)
5 ... Yoshihara, Mizuno: Mode I Critical Stress Intensity Factor of MediumDensity... and (3) (4) The appropriate value of additional crack length was determined from the following procedure, which was similar to those conducted in previous studies (Yoshihara, 2010a, b; Yoshihara and Usuki, 2011). By altering the value of, the probability value (pvalue) for the averages of KIc obtained by the SENB test corresponding to each a/w and DCB test is calculated by Student s ttest. Then the pvalues corresponding to each are summed up. When the amount of the pvalues is large, the average values of KIc obtained by the SENB and DCB tests can be regarded as being close to each other. The value was obtained by binary search algorithm as shown in Table 1. The values listed in Table 1 are longer than those of western hemlock, which were 2 and 4 mm for specimen A and B, respectively (Yoshihara, 2010a). Table 1 Additional crack length derived by statistically comparing K Ic values obtained from SENB and DCB tests (unit = mm) Tablica 1. Dodatna duljina pukotine dobivena statističkom usporedbom vrijednosti K Ic ustanovljene SENB testom i DCB testom (jedinica mm) W Equation Relationship / Odnos Jednadžba Pδ PCOD 20 (3) (4) (3) (4) The value obtained from the PCOD relationship is larger than that obtained from the Pδ relationship. Figure 3 also shows the results calculated by Eqs. (3) and (4). The values of K Ic obtained from Eq. (3) are close to those obtained by the DCB tests when a/w falls in the approximate range of 0.5 to 0.7. A statistical analysis of the difference between the K Ic values obtained using the SENB and DCB tests shows that the difference is not significant in this a/w range, regardless of whether the P c value is determined from the Pδ or PCOD relationship. This range coincides well with the range used to derive the appropriate K Ic value in the SENT test (Yoshihara 2010b). When using Eq. (4), however, the applicable range of a/w is narrower than that obtained using Eq. (3). When the a/w value is smaller than 0.4, material nonlinearity precedes the crack propagation, so the load at the onset of nonlinearity in the Pδ and PCOD relationships P c cannot be regarded as the critical load for crack propagation (Yoshihara 2010b). Therefore, the K Ic values for a/w values smaller than 0.4 were measured to be smaller than those in the a/w range from 0.5 to 0.7. In contrast, the value of K Ic calculated from Eq. (3) decreases in the a/w range larger than 0.8, whereas that calculated from Eq. (4) diverges when a/w exceeds 0.8 because the value of 1  (a + )/W contained in the equation is close to zero. Therefore, the K Ic a/w relationships obtained from Eqs. (3) and (4) are extremely different from each other when the value of a/w exceeds 0.8. Additionally, when the crack tip is close to the loading point, the compressive stresses due to the indentation of the loading nose hinder selfsimilar crack propagation (de Moura et al., 2010). From these reasons, the appropriate range for introducing the additional crack is restricted. From the results obtained here, the K Ic value should be measured using Eq. (3) in the a/w range from 0.5 to 0.7. In this research, the additional crack length is determined by statistically comparing the K Ic values obtained from the Pδ and PCOD relationships and that obtained by the DCB test. Therefore, the value is dependent on the relationship used in the analysis, as shown in Table 1. Based on the concept of the FPZ, however, the value of can be physically obtained (Vasic and Smith, 2002; Vasic et al., 2003; Morel et al., 2003; 2005; de Moura et al., 2008, 2010; Dourado et al., 2008, 2010). As shown in Figure 2, the K Ic values obtained from both Pδ and PCOD relationships are similar to each other when correcting the crack length. Therefore, it is difficult to determine which relationship is more valid for determining the K Ic value. Microscopic observation (Vasic and Smith, 2002; Vasic et al., 2003) and digital image correlation observation (Murata et al., 2011) around the crack tip during loading may be effective to reveal the validity of the relationships. According to the research on the Mode II critical stress intensity factor K IIc of wood and MDF as determined by an asymmetric fourpoint bending test, the K IIc value can be obtained by introducing the additional crack length when a/w exceeds 0.8, when an appropriate equation is derived for the crack geometry factor (Yoshihara submitted). In the SENB tests of solid wood (Yoshihara, 2010a) and MDF, two previously proposed equations (Eqs. (1) and (2)) were used and modified by considering the additional crack length. Further research should be conducted to find a new equation that can derive the K Ic value properly for the specimen with an a/w value larger than 0.8. In addition, the compressive stresses due to the indentation of the loading nose DRVNA INDUSTRIJA 65 (2) (2014) 103
6 Yoshihara, Mizuno: Mode I Critical Stress Intensity Factor of MediumDensity can be reduced when conducting the fourpoint SENB (4SENB) test in which the loadingline deviates from the crack pass, and the range of a/w can be extended. Therefore, further research should also be conducted on the 4SENB test of MDF and solid wood. 4 CONCLUSIONS 4. ZAKLJUČAK A singleedgenotched bending (SENB) test of MDF was conducted to obtain the Mode I critical stress intensity factor K Ic. The test results were compared with those of the double cantilever beam (DCB) tests, an approach that is thought to be valid because the K Ic value can be determined based on energy considerations. The above results are interpreted to indicate that the critical stress intensity factor K Ic in Mode I can be obtained effectively by introducing the additional crack length as in Eq. (3) under the range of the crack length/specimen depth ratio a/w from 0.5 to 0.7. This range coincided well with that obtained in the singleedgenotched tension (SENT) tests of MDF Yoshihara, 2010b). To determine the value of K Ic under a wide range of a/w, further research should be undertaken on issues such as additional crack lengths, other equations for determining the K Ic value, and other test methods including the fourpoint SENB (4SENB) test. Acknowledgement  Zahvala This work was supported in part by a Grantin Aid for Scientific Research (C) (No ) from the Japan Society for the Promotion of Science (JSPS). 5 REFERENCES 5. LITERATURA 1. Adams, D. F.; Carlsson, L. A.; Pipes, R. B., 2003: Experimental Characterization of Advanced Composites Materials. 3rd edition, Boca Raton: CRC Press 2. De Moura, M. F. S. F.; Morais, J. J. L.; Dourado, N., 2008: A new data reduction scheme for mode I wood fracture characterization using the double cantilever beam test. Engineering Fracture Mechanics 75 (13): De Moura, M. F. S. F.; Dourado, N.; Morais, J. J. L., 2010: Crack equivalent based method applied to wood fracture characterization using the single edge notchedthree point bending test. Engineering Fracture Mechanics 77 (3): Dourado, N.; Morel, S.; de Moura, M. F. S. F.; Valentin, G.; Morais, J., 2008: Comparison of fracture properties of two wood species through cohesive crack simulations. Composites Part A: Applied Science and Manufacturing 39 (2): Dourado, N. M. M.; de Moura, M. F. S. F.; Morais, J. J. L.; Silva, M. A. L., 2010: Estimate of resistancecurve in wood through the double cantilever beam test. Holzforschung 64 (1): Morel, S.; Bouchaud, E.; Schmittbuhl, J., 2003: Influence of the specimen geometry on Rcurve behavior and roughening of fracture surfaces. International Journal of Fracture 121 (12): Morel, S.; Dourado, N.; Valentin, G.; Morais, J., 2005: Wood: a quasibrittle material Rcurve behavior and peak load evaluation. International Journal of Fracture 131 (4): Murata, K.; Nagai, H.; Nakano, T., 2011: Estimation of width of fracture process zone in spruce wood by radial tensile test. Mechanics of Materials 43 (7): Vasic, S.; Smith, I., 2002: Bridging crack model for fracture of spruce. Engineering Fracture Mechanics 69 (6): Vasic, S.; Smith, I.; Landis, E., 2003: Fracture zone characterization. Micromechanical study. Wood and Fiber Science 34 (1): Yoshihara, H., 2010a: Examination of the mode I critical stress intensity factor of wood obtained by singleedgenotched bending test. Holzforschung 64 (4): Yoshihara, H., 2010b: Influence of loading conditions on the measurement of mode I critical stress intensity factor for wood and mediumdensity fiberboard by the singleedgenotched tension test. Holzforschung 64 (6): Yoshihara, H.; Usuki, A., 2011: Mode I critical stress intensity factor of wood and mediumdensity fibreboard measured by compact tension test. Holzforschung 65 (5): Yoshihara, H., 2013: Mode II critical stress intensity factor of mediumdensity fiberboard measured by asymmetric fourpoint bending tests and analyses of kink crack formation. BioResources 8 (2): Corresponding address: Professor HIROSHI YOSHIHARA, Ph.D. Shimane University Faculty of Science and Engineering Nishikawazucho 1060 Matsue, Shimane , JAPAN DRVNA INDUSTRIJA 65 (2) (2014)
Shear Modulus and Shear Strength Evaluation of Solid Wood by a Modified ISO SquarePlate Twist Method
Hiroshi Yoshihara 1 Shear Modulus and Shear Strength Evaluation of Solid Wood by a Modified ISO 1531 Squarelate Twist Method rocjena smicajnog modula i smicajne čvrstoće cjelovitog drva modificiranom
More informationA NEW METHODOLOGY FOR THE CHARACTERIZATION OF MODE II FRACTURE OF PINUS PINASTER WOOD
5th International Conference on Mechanics and Materials in Design REF: A0604.009 (Invited Paper) A NEW METHODOLOY FOR THE CHARACTERIZATION OF MODE II FRACTURE OF PINUS PINASTER WOOD M.F.S.F. de Moura 1*,
More informationESCOLA POLITÉCNICA DA UNIVERSIDADE DE SÃO PAULO BOLETIM TÉCNICO PEFEPUSP. Título:
ESCOLA POLITÉCNICA DA UNIVERSIDADE DE SÃO PAULO BOLETIM TÉCNICO PEFEPUSP Título: STUDY OF CRACK PROPAGATION IN THE SPECIMEN RECOMMENDED BY RILEM TC 16 BASED ON LINEAR ELASTIC FRACTURE MECHANICS LUIZ EDUARDO
More informationSimple estimation of critical stress intensity factors of wood by tests with double cantilever beam and threepoint endnotched flexure
Holzforschung, Vol. 6, pp. 8 89, 007 Copright b Walter de Gruter Berlin New York. DO 0.55/HF.007.0 Simple estimation of critical stress intensit factors of wood b tests with double cantilever beam and
More informationMixedMode Fracture Toughness Determination USING NONCONVENTIONAL TECHNIQUES
MixedMode Fracture Toughness Determination USING NONCONVENTIONAL TECHNIQUES IDMEC Pólo FEUP DEMec  FEUP ESM Virginia Tech motivation fracture modes conventional tests [mode I] conventional tests [mode
More informationWOOD FRACTURE PATTERN DURING THE WATER DESORPTION PROCESS ABSTRACT
ISSN 07173644 ISSN online 0718221X Maderas. Ciencia y tecnología 8(1): 2530, 2006 WOOD FRACTURE PATTERN DURING THE WATER DESORPTION PROCESS Liyu Wang 1, Guangjie Zhao 2, Zhenyou Lu 3 ABSTRACT Wood is
More informationOn characterising fracture resistance in modei delamination
9 th International Congress of Croatian Society of Mechanics 1822 September 2018 Split, Croatia On characterising fracture resistance in modei delamination Leo ŠKEC *, Giulio ALFANO +, Gordan JELENIĆ
More informationCOMPARISON OF MODULY OF ELASTICITY OBTAINED BY NON DESTRUCTIVE AND DESTRUCTIVE TESTS OF TIMBER SAMPLES
COMPARISON OF MODULY OF ELASTICITY OBTAINED BY NON DESTRUCTIVE AND DESTRUCTIVE TESTS OF TIMBER SAMPLES Marta Čukman University of Zagreb, Faculty of Civil Engineering, student Corresponding author: marta.cukman@gmail.com
More informationCharacterization of Fiber Bridging in Mode II Fracture Growth of Laminated Composite Materials
Applied Mechanics and Materials Online: 20100630 ISSN: 16627482, Vols. 2425, pp 245250 doi:10.4028/www.scientific.net/amm.2425.245 2010 Trans Tech Publications, Switzerland Characterization of Fiber
More informationMassachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139
Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139 2.002 Mechanics and Materials II Spring 2004 Laboratory Module No. 6 Fracture Toughness Testing and Residual
More informationEXPERIMENTBASED CRITERION FOR THE CRACK STABILITY ANALYSIS IN COMPOSITE MATERIALS
Gépészet 008 Budapest, 90.May 008. G008J04 EXPERIMENTBASED CRITERION FOR THE CRACK STABILITY ANALYSIS IN COMPOSITE MATERIALS András Szekrényes Assistant Professor, Department of Applied Mechanics,
More informationFig. 1. Different locus of failure and crack trajectories observed in mode I testing of adhesively bonded double cantilever beam (DCB) specimens.
a). Cohesive Failure b). Interfacial Failure c). Oscillatory Failure d). Alternating Failure Fig. 1. Different locus of failure and crack trajectories observed in mode I testing of adhesively bonded double
More informationCHARACTERIZATION OF ROTATIONAL BEHAVIOR OF WEBFLANGE JUNCTIONS OF PULTRUDED GFRP BRIDGE DECKS
CHARACTERIZATION OF ROTATIONAL BEHAVIOR OF WEBFLANGE JUNCTIONS OF PULTRUDED GFRP BRIDGE DECKS S. YanesArmas, J. De Castro and T. Keller Composite Construction Laboratory (CCLab), Ecole Polytechique Fédérale
More informationFinite Element Analysis of FRP Debonding Failure at the Tip of Flexural/Shear Crack in Concrete Beam
Marquette University epublications@marquette Civil and Environmental Engineering Faculty Research and Publications Civil and Environmental Engineering, Department of 1212013 Finite Element Analysis
More informationFRACTURE IN PBX 9501 AT LOW RATES
FRACTURE IN PBX 9501 AT LOW RATES Cheng Liu & Richard Browning Los Alamos National Laboratory Los Alamos, NM 87545 Tensile, or mode I, fractures in PBX 9501 have a very large process zone that runs well
More informationStrainsoftening behavior of wood under tension perpendicular to the grain
J Wood Sci (7) 53:63 69 The Japan Wood Research Society 7 DOI.7/s67993 ORIGINAL ARTICLE Kazunari Miyauchi Koji Murata softening behavior of wood under tension perpendicular to the grain Received: November,
More informationStandard Test Methods for PlaneStrain Fracture Toughness and Strain Energy Release Rate of Plastic Materials 1
Designation: D 5045 99 AMERICAN SOCIETY FOR TESTING AND MATERIALS 100 Barr Harbor Dr., West Conshohocken, PA 19428 Reprinted from the Annual Book of ASTM Standards. Copyright ASTM Standard Test Methods
More informationLecture #7: Basic Notions of Fracture Mechanics Ductile Fracture
Lecture #7: Basic Notions of Fracture Mechanics Ductile Fracture by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering, Chair of Computational Modeling of Materials in Manufacturing
More informationEffect of board density on bending properties and dimensional stabilities of MDFreinforced corrugated particleboard
J Wood Sci (2003) 49:398 404 The Japan Wood Research Society 2003 DOI 10.1007/s100860020501y ORIGINAL ARTICLE Koji Hayashi Masaharu Ohmi Hiroshi Tominaga Kiyoharu Fukuda Effect of board density on bending
More informationDetermination of sizeindependent specific fracture energy of concrete from threepoint bend and wedge splitting tests
Magazine of Concrete Research, 3, 55, No. 2, April, 133 141 Determination of sizeindependent specific fracture energy of concrete from threepoint bend and wedge splitting tests H. M. Abdalla and B. L.
More informationEDEM DISCRETIZATION (Phase II) Normal Direction Structure Idealization Tangential Direction Pore spring Contact spring SPRING TYPES Inner edge Inner d
Institute of Industrial Science, University of Tokyo Bulletin of ERS, No. 48 (5) A TWOPHASE SIMPLIFIED COLLAPSE ANALYSIS OF RC BUILDINGS PHASE : SPRING NETWORK PHASE Shanthanu RAJASEKHARAN, Muneyoshi
More informationBilinear softening parameters and equivalent LEFM Rcurve in quasibrittle failure
Bilinear softening parameters and equivalent LEFM Rcurve in quasibrittle failure S. Morel, C. Lespine, J.L Coureau, J. Planas, N. Dourado Université Bordeaux, US2B (UMR 503), 35 cours de la Liberation,
More informationEffect of Thermal Treatment on Fracture Properties and Adsorption Properties of Spruce Wood
Materials 2013, 6, 41864197; doi:10.3390/ma6094186 Article OPEN ACCESS materials ISSN 19961944 www.mdpi.com/journal/materials Effect of Thermal Treatment on Fracture Properties and Adsorption Properties
More informationSTRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS
STRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS By Joseph F. Murphy 1 ABSTRACT: Four large glulam beams with notches on the tension side were tested for strength and stiffness. Using either bending
More informationPOSTPEAK BEHAVIOR OF FRPJACKETED REINFORCED CONCRETE COLUMNS
POSTPEAK BEHAVIOR OF FRPJACKETED REINFORCED CONCRETE COLUMNS  Technical Paper  Tidarut JIRAWATTANASOMKUL *1, Dawei ZHANG *2 and Tamon UEDA *3 ABSTRACT The objective of this study is to propose a new
More informationEvaluation of inplane orthotropic elastic constants of paper and paperboard
Evaluation of inplane orthotropic elastic constants of paper and paperboard T. Yokoyama and K. Nakai Department of Mechanical Engineering, Okayama University of Science  Ridaicho, Okayama 75, Japan
More informationDEPARTMENT OF MECHANICAL ENIGINEERING, UNIVERSITY OF ENGINEERING & TECHNOLOGY LAHORE (KSK CAMPUS).
DEPARTMENT OF MECHANICAL ENIGINEERING, UNIVERSITY OF ENGINEERING & TECHNOLOGY LAHORE (KSK CAMPUS). Lab Director: Coordinating Staff: Mr. Muhammad Farooq (Lecturer) Mr. Liaquat Qureshi (Lab Supervisor)
More informationEVALUATION OF MODULUS OF RIGIDITY BY DYNAMIC PLATE SHEAR TESTING Tetsuya Nakao. and Takeshi Okano
EVALUATION OF MODULUS OF RIGIDITY BY DYNAMIC PLATE SHEAR TESTING Tetsuya Nakao Graduate Student Present address: Department of Forestry Faculty of Agriculture Shimane University Matsue 690, Japan and Takeshi
More informationMEASURMENT OF BENDING PROPERTIES OF RHIZOPHORA TROPICAL WOOD. Sarawak, Malaysia. Engineering & Technology, Dhaka, Bangladesh
AJSTD Vol. 26 Issue 2 pp. 7384 (2010) MEASURMENT OF BENDING PROPERTIES OF RHIZOPHORA TROPICAL WOOD Sinin Hamdan* a, Mahbub Hasan b and Yoann Nohe c a Faculty of Engineering, Universiti Malaysia Sarawak,
More informationUNIT III DEFLECTION OF BEAMS 1. What are the methods for finding out the slope and deflection at a section? The important methods used for finding out the slope and deflection at a section in a loaded
More informationAnalytical and Numerical Modeling of R Curves for Cracks with Bridging Zones
International Journal of Fracture volume 5, number 2, 167 181 (29) Analytical and Numerical Modeling of R Curves for Cracks with Bridging Zones John A. Nairn Received: 13 June 28 / Accepted: 16 March 29
More informationModeling of Interfacial Debonding Induced by IC Crack for Concrete Beambonded with CFRP
Proceedings of the World Congress on Engineering 21 Vol II WCE 21, June 2  July 1, 21, London, U.K. Modeling of Interfacial Debonding Induced by IC Crack for Concrete Beambonded with CFRP Lihua Huang,
More information> Buy TruePDF > Autodelivered in 0~10 minutes. GB/T Translated English of Chinese Standard: GB/T
Translated English of Chinese Standard: GB/T41612007 www.chinesestandard.net Buy TruePDF Autodelivery. Sales@ChineseStandard.net ICS 77.040.10 NATIONAL STANDARD OF THE PEOPLE S REPUBLIC OF CHINA GB
More informationAnalysis of CantileverBeam Bending Stress Relaxation Properties of Thin Wood Composites
Analysis of CantileverBeam Bending Stress Relaxation Properties of Thin Wood Composites John F. Hunt, a, * Houjiang Zhang, b and Yan Huang b An equivalent strain method was used to analyze and determine
More informationSpecial edition paper
Development of New Aseismatic Structure Using Escalators Kazunori Sasaki* Atsushi Hayashi* Hajime Yoshida** Toru Masuda* Aseismatic reinforcement work is often carried out in parallel with improvement
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationAutodesk Helius PFA. Guidelines for Determining Finite Element Cohesive Material Parameters
Autodesk Helius PFA Guidelines for Determining Finite Element Cohesive Material Parameters Contents Introduction...1 Determining Cohesive Parameters for Finite Element Analysis...2 What Test Specimens
More informationFRACTURE MECHANICS TEST METHODS
DEVELOPMENT AND EVALUATION OF FRACTURE MECHANICS TEST METHODS FOR SANDWICH COMPOSITES Dan Adams Department of Mechanical Engineering University it of Utah Salt Lake City, UT AMTAS A t 2012 M ti AMTAS Autumn
More informationPlasticity Analysis of the Strain in the Tangential Direction of Solid Wood Subjected to Compression Load in the Longitudinal Direction
Plasticity Analysis of the Strain in the Tangential Direction of Solid Wood Subjected to Compression Load in the Longitudinal Direction Hiroshi Yoshihara Uniaxial compression tests in the grain (longitudinal)
More informationNUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET
NUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET M.Gümüş a*, B.Gözlüklü a, D.Çöker a a Department of Aerospace Eng., METU, Ankara, Turkey *mert.gumus@metu.edu.tr Keywords:
More informationElasticPlastic Fracture Mechanics. Professor S. Suresh
ElasticPlastic Fracture Mechanics Professor S. Suresh Elastic Plastic Fracture Previously, we have analyzed problems in which the plastic zone was small compared to the specimen dimensions (small scale
More informationFracture Mechanics, Damage and Fatigue Non Linear Fracture Mechanics: JIntegral
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue Non Linear Fracture Mechanics: JIntegral Ludovic Noels Computational & Multiscale Mechanics of Materials CM3
More informationRELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer
RELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer and Robert J. Ross Supervisory Research Engineer USDA Forest Service Forest Products
More informationPRO LIGNO Vol. 14 N pp. 38
ELASTIC CONSTANTS OF MDF CORE AND FACE LAYERS DETERMINED BY COMPRESSION TESTS Ergün GÜNTEKIN Department of Forest Products Engineering, Faculty of Forestry, Suleyman Demirel University 32260 Isparta, Turkey
More informationThe Effects of Transverse Shear on the Delamination of EdgeNotch Flexure and 3Point Bend Geometries
The Effects of Transverse Shear on the Delamination of EdgeNotch Flexure and 3Point Bend Geometries M. D. Thouless Department of Mechanical Engineering Department of Materials Science & Engineering University
More informationCHAPTER 3 EXPERIMENTAL STUDY
Experimental Study 42 CHAPTER 3 EXPERIMENTAL STUDY 3.1. INTRODUCTION The experimental study that has been carried out in this thesis has two main objectives: 1. Characterise the concrete behaviour in mode
More informationINFLUENCE OF LOADING RATIO ON QUANTIFIED VISIBLE DAMAGES OF R/C STRUCTURAL MEMBERS
Paper N 1458 Registration Code: SH1463506048 INFLUENCE OF LOADING RATIO ON QUANTIFIED VISIBLE DAMAGES OF R/C STRUCTURAL MEMBERS N. Takahashi (1) (1) Associate Professor, Tohoku University, ntaka@archi.tohoku.ac.jp
More informationFracture Behavior. Section
Section 6 Fracture Behavior In January 1943 the oneday old Liberty Ship, SS Schenectady, had just completed successful sea trials and returned to harbor in calm cool weather when... "Without warning and
More informationNational Exams May 2015
National Exams May 2015 04BS6: Mechanics of Materials 3 hours duration Notes: If doubt exists as to the interpretation of any question, the candidate is urged to submit with the answer paper a clear
More informationStandard Test Methods for PlaneStrain Fracture Toughness and Strain Energy Release Rate of Plastic Materials 1
This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards,
More informationFlexural properties of polymers
A2 _EN BUDAPEST UNIVERSITY OF TECHNOLOGY AND ECONOMICS FACULTY OF MECHANICAL ENGINEERING DEPARTMENT OF POLYMER ENGINEERING Flexural properties of polymers BENDING TEST OF CHECK THE VALIDITY OF NOTE ON
More informationA new approach for investigation of damage zone properties in orthotropic materials
Engineering Solid Mechanics 2 (214) 283292 Contents lists available at GrowingScience Engineering Solid Mechanics homepage: www.growingscience.com/esm A new approach for investigation of damage zone properties
More informationMMJ1133 FATIGUE AND FRACTURE MECHANICS E ENGINEERING FRACTURE MECHANICS
E ENGINEERING WWII: Liberty ships Reprinted w/ permission from R.W. Hertzberg, "Deformation and Fracture Mechanics of Engineering Materials", (4th ed.) Fig. 7.1(b), p. 6, John Wiley and Sons, Inc., 1996.
More informationMODELING OF THE WEDGE SPLITTING TEST USING AN EXTENDED CRACKED HINGE MODEL
Engineering MECHANICS, Vol. 21, 2014, No. 1, p. 67 72 67 MODELING OF THE WEDGE SPLITTING TEST USING AN EXTENDED CRACKED HINGE MODEL Tomáš Pail, Petr Frantík* The present paper describes a semianalytical
More informationEngineering Fracture Mechanics 74 (2007) Elsevier Ltd, doi: /j.engfracmech
Engineering Fracture Mechanics 74 (007) 771781 Elsevier Ltd, doi: 101016/j.engfracmech.006.06.015 A new fracture mechanics theory of orthotropic materials like wood T.A.C.M. van der Put, TUDelft, CiTG,
More informationMethod of test for fracture energy of concrete by use of notched beam JCIS
Japan Concrete Institute Standard Method of test for fracture energy of concrete by use of notched beam JCIS0012003 1. Scope This test method covers determination of fracture energy of concrete (1)
More informationPresented by: Civil Engineering Academy
Presented by: Civil Engineering Academy Structural Design and Material Properties of Steel Presented by: Civil Engineering Academy Advantages 1. High strength per unit length resulting in smaller dead
More informationFRACTURE MECHANICS FOR MEMBRANES
FRACTURE MECHANICS FOR MEMBRANES Chong Li, Rogelio Espinosa and Per Ståhle Solid Mechanics, Malmö University SE 205 06 Malmö, Sweden chong.li@ts.mah.se Abstract During fracture of membranes loading often
More informationCRACK growth in continuous fiber ceramic composites (CFCCs)
journal J. Am. Ceram. Soc., 87 [5] 914 922 (2004) Notch Sensitivity of Ceramic Composites with Rising Fracture Resistance Michael A. Mattoni* and Frank W. Zok* Materials Department, University of California,
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More information2012 MECHANICS OF SOLIDS
R10 SET  1 II B.Tech II Semester, Regular Examinations, April 2012 MECHANICS OF SOLIDS (Com. to ME, AME, MM) Time: 3 hours Max. Marks: 75 Answer any FIVE Questions All Questions carry Equal Marks ~~~~~~~~~~~~~~~~~~~~~~
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationFHWA Bridge Design Guidance No. 1 Revision Date: July 21, Load Rating Evaluation of Gusset Plates in Truss Bridges
FHWA Bridge Design Guidance No. 1 Revision Date: July 21, 2008 Load Rating Evaluation of Gusset Plates in Truss Bridges By Firas I. Sheikh Ibrahim, PhD, PE Part B Gusset Plate Resistance in Accordance
More informationPROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING. C. G. Dávila, P. P. Camanho, and M. F. de Moura
PROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING C. G. Dávila, P. P. Camanho, and M. F. de Moura Abstract The debonding of skin/stringer constructions is analyzed using a stepbystep simulation
More informationAcoustic emission analysis for failure identification in composite materials
Acoustic emission analysis for failure identification in composite materials Markus G. R. Sause Experimental Physics II Institute of Physics University of Augsburg 1. Motivation 2. Methods of AE analysis
More informationDEVELOPMENT OF TEST GUIDANCE FOR COMPACT TENSION FRACTURE TOUGHNESS SPECIMENS CONTAINING NOTCHES INSTEAD OF FATIGUE PRECRACKS
Transactions, SMiRT23 Division II, Paper ID 287 Fracture Mechanics and Structural Integrity DEVELOPMENT OF TEST GUIDANCE FOR COMPACT TENSION FRACTURE TOUGHNESS SPECIMENS CONTAINING NOTCHES INSTEAD OF
More informationFinal Analysis Report MIE 313 Design of Mechanical Components
Final Analysis Report MIE 313 Design of Mechanical Components Juliana Amado Charlene Nestor Peter Walsh Table of Contents Abstract:...iii Introduction:... 4 Procedure:... 5 Results:... 6 Reliability:...
More informationProject MMS13 Task 5 Report No 3 (M6/D3)
Project MMS13 Task 5 Report No 3 (M6/D3) Material Data Requirements and Recommended Test Methods for the Predictive Modelling of Defect Criticality in Composite Material Systems M R L Gower and G D Sims
More informationSize effect in the strength of concrete structures
Sādhanā Vol. 27 Part 4 August 2002 pp. 449 459. Printed in India Size effect in the strength of concrete structures B L KARIHALOO and Q Z XIAO Division of Civil Engineering School of Engineering Cardiff
More informationFRACTURE IN HIGH PERFORMANCE FIBRE REINFORCED CONCRETE PAVEMENT MATERIALS
FRACTURE IN HIGH PERFORMANCE FIBRE REINFORCED CONCRETE PAVEMENT MATERIALS ERIK DENNEMAN A thesis submitted in partial fulfilment of the requirements for the degree of PHILOSOPHIAE DOCTOR (ENGINEERING)
More informationExperimentally Calibrating Cohesive Zone Models for Structural Automotive Adhesives
Experimentally Calibrating Cohesive Zone Models for Structural Automotive Adhesives Mark Oliver October 19, 2016 Adhesives and Sealants Council Fall Convention contact@veryst.com www.veryst.com Outline
More informationNONLINEAR FRACTURE BEHAVIOR OF DOUBLE CANTILEVER BEAM
Engineering MECHANICS, Vol., 015, No., p. 95 10 95 NONLINEAR FRACTURE BEHAVIOR OF DOUBLE CANTILEVER BEAM Viktor Rizov* This article describes a theoretical study of nonlinear fracture behavior of the
More informationComparative study of fracture mechanical test methods for concrete
Comparative study of fracture mechanical test methods for concrete Lennart Østergaard & John Forbes Olesen Department of Civil Engineering, Technical University of Denmark,. Brovej, Building 118, DK2800
More informationSimulation of Geometrical CrossSection for Practical Purposes
Simulation of Geometrical CrossSection for Practical Purposes Bhasker R.S. 1, Prasad R. K. 2, Kumar V. 3, Prasad P. 4 123 Department of Mechanical Engineering, R.D. Engineering College, Ghaziabad, UP,
More informationExperimental Study and Numerical Simulation on Steel Plate Girders With Deep Section
6 th International Conference on Advances in Experimental Structural Engineering 11 th International Workshop on Advanced Smart Materials and Smart Structures Technology August 12, 2015, University of
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationDesign of AAC wall panel according to EN 12602
Design of wall panel according to EN 160 Example 3: Wall panel with wind load 1.1 Issue Design of a wall panel at an industrial building Materials with a compressive strength 3,5, density class 500, welded
More informationCOMPARISON BETWEEN TENSILE AND COMPRESSIVE YOUNG S MODULUS OF STRUCTURAL SIZE LUMBER
COMPARISON BETWEEN TENSILE AND COMPRESSIVE YOUNG S MODULUS OF STRUCTURAL SIZE LUMBER KwangMo Kin 1, KugBo Shim 2 ABSTRACT: To evaluate MOE of glued laminated timber, usually nondestructive MOE values
More informationBy Dr. Mohammed Ramidh
Engineering Materials Design Lecture.6 the design of beams By Dr. Mohammed Ramidh 6.1 INTRODUCTION Finding the shear forces and bending moments is an essential step in the design of any beam. we usually
More informationSabah Shawkat Cabinet of Structural Engineering Walls carrying vertical loads should be designed as columns. Basically walls are designed in
Sabah Shawkat Cabinet of Structural Engineering 17 3.6 Shear walls Walls carrying vertical loads should be designed as columns. Basically walls are designed in the same manner as columns, but there are
More informationA NEW SIMPLIFIED AND EFFICIENT TECHNIQUE FOR FRACTURE BEHAVIOR ANALYSIS OF CONCRETE STRUCTURES
Fracture Mechanics of Concrete Structures Proceedings FRAMCOS3 AEDFCATO Publishers, D79104 Freiburg, Germany A NEW SMPLFED AND EFFCENT TECHNQUE FOR FRACTURE BEHAVOR ANALYSS OF CONCRETE STRUCTURES K.
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationTreatment of Constraint in NonLinear Fracture Mechanics
Treatment of Constraint in NonLinear Fracture Mechanics Noel O Dowd Department of Mechanical and Aeronautical Engineering Materials and Surface Science Institute University of Limerick Ireland Acknowledgements:
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More informationNumerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive Zone Model
Numerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive Zone Model Numerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive
More informationChapter 8. Shear and Diagonal Tension
Chapter 8. and Diagonal Tension 8.1. READING ASSIGNMENT Text Chapter 4; Sections 4.14.5 Code Chapter 11; Sections 11.1.1, 11.3, 11.5.1, 11.5.3, 11.5.4, 11.5.5.1, and 11.5.6 8.2. INTRODUCTION OF SHEAR
More informationFracture mechanics analysis of arc shaped specimens for pipe grade polymers
Fracture mechanics analysis of arc shaped specimens for pipe grade polymers Pemra Özbek, Christos Argyrakis and Patrick Leevers Department of Mechanical Engineering, Imperial College London, London SW7
More informationValidity of fracture mechanics concepts applied to wood by finite element calculation
Wood Sci. Technol. 18:5158 (1984) Wood Science and Technology 9 SpringerVerlag 1984 Validity of fracture mechanics concepts applied to wood by finite element calculation P. Triboulot*, Champenoux, P.
More informationStress Analysis Lecture 4 ME 276 Spring Dr./ Ahmed Mohamed Nagib Elmekawy
Stress Analysis Lecture 4 ME 76 Spring 017018 Dr./ Ahmed Mohamed Nagib Elmekawy Shear and Moment Diagrams Beam Sign Convention The positive directions are as follows: The internal shear force causes a
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationExperimental characterization of interlaminar fracture toughness of composite laminates assembled with three different carbon fiber lamina
Experimental characterization of interlaminar fracture toughness of composite laminates assembled with three different carbon fiber lamina Domenico Gentile University of Cassino and Southern Lazio, Cassino
More informationMoment redistribution of continuous composite Igirders with high strength steel
Moment redistribution of continuous composite Igirders with high strength steel * Hyun Sung Joo, 1) Jiho Moon, 2) IkHyun sung, 3) HakEun Lee 4) 1), 2), 4) School of Civil, Environmental and Architectural
More informationELECIRONIC SPECKLE PATTERN INTERFEROMETRY IN CHARACTERIZING
ELECIRONIC SPECKLE PATTERN INTERFEROMETRY IN CHARACTERIZING ROCK FRACTURE A. K. Maji and J. L. Wang Department of Civil Engineering University of New Mexico Albuquerque, NM 87131 INTRODUCTION The fracture
More informationCOMPARISON OF THE SIZEINDEPENDENT FRACTURE ENERGY OF CONCRETE OBTAINED BY TWO TEST METHODS
VIII International Conference on Fracture Mechanics of Concrete and Concrete Structures FraMCoS8 J.G.M. Van Mier, G. Ruiz, C. Andrade, R.C. Yu and X.X. Zhang (Eds) COMPARISON OF THE SIZEINEPENENT FRACTURE
More informationNUMERICAL AND EXPERIMENTAL ANALYSES OF MULTIPLE DELAMINATIONS IN CURVED COMPOSITE LAMINATES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS NUMERICAL AND EXPERIMENTAL ANALYSES OF MULTIPLE DELAMINATIONS IN CURVED COMPOSITE LAMINATES A. Baldi 1 *, A. Airoldi 1, P. Belotti 1, P. Bettini
More informationAPPLICATION OF INTENSIVE SHEAR REINFORCEMENT TO SPLICING SLEEVE JOINT OF PREFABRICATED REINFORCEMENT ASSEMBLY
13 th World Conference on Earthquake Engineering Vancouver, B.C., Canada August 16, 24 Paper No. 587 APPLICATION OF INTENSIVE SHEAR REINFORCEMENT TO SPLICING SLEEVE JOINT OF PREFABRICATED REINFORCEMENT
More informationSRI VIDYA COLLEGE OF ENGINEERING AND TECHNOLOGY, VIRUDHUNAGAR CE 6602 STRUCTURAL ANALYSIS  II DEPARTMENT OF CIVIL ENGINEERING CE 6501 STRUCTURAL ANALYSIS  I 2 MARK QUESTION BANK UNIT II  INFLUENCE LINES
More informationEFFECT OF SHEAR REINFORCEMENT ON FAILURE MODE OF RC BRIDGE PIERS SUBJECTED TO STRONG EARTHQUAKE MOTIONS
EFFECT OF SHEAR REINFORCEMENT ON FAILURE MODE OF RC BRIDGE PIERS SUBJECTED TO STRONG EARTHQUAKE MOTIONS Atsuhiko MACHIDA And Khairy H ABDELKAREEM SUMMARY Nonlinear D FEM was utilized to carry out inelastic
More information5 ADVANCED FRACTURE MODELS
Essentially, all models are wrong, but some are useful George E.P. Box, (Box and Draper, 1987) 5 ADVANCED FRACTURE MODELS In the previous chapter it was shown that the MOR parameter cannot be relied upon
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More information